Download presentation

Presentation is loading. Please wait.

Published byJordon O'Neal Modified about 1 year ago

1
Chapter 13 Creep and Superplasticity

2
Creep Strain vs.Time: Constant Temperature

3
Creep Strain vs. Time at Constant Engineering Stress

4
Creep machine with variable lever arms to ensure constant stress on specimen; note that l2 decreases as the length of the specimen increases. Creep Machine Initial position Length of specimen has increased from L0 to L1.

5
Mukherjee-Bird-Dorn Equation

6
Relationship between time to rupture and temperature at three levels of engineering stress, σa, σb, and σc, using Larson–Miller equation (σa > σb > σc). Larson-Miller Equation

7
Master plot for Larson–Miller parameter for S-590 alloy (an Fe-based alloy) (C = 17). (From R. M. Goldhoff, Mater.Design Eng., 49 (1959) 93.) Larson-Miller Parameter

8
Relationship between time rupture and temperature at three levels of stress, σa, σb, and σc, using Manson–Haferd parameter (σa > σb > σc). Manson-Hafered Parameter

9
Relationship between time to rupture and temperature at three levels of stress, σa > σb > σc, using Sherby– Dorn parameter. Sherby-Dorn Parameter

10
Material Parameters

11
Activation energies for creep (stage II) and self-diffusion for a number of metals. (Adapted with permission from O. D. Sherby and A. K. Miller, J. Eng. Mater.Technol., 101 (1979) 387.) Activation Energies for Creep

12
Ratio between activation energy for secondary creep and activation energy for bulk diffusion as a function of temperature. (Adapted with permission from O. D. Sherby and A. K. Miller, J. Eng. Mater. Technol., 101 (1979) 387.) Secondary Creep

13
Fundamental Creep Mechanism σ/G < 10^(-4) Diffusion Creep –Nabarro Herring –Coble Creep –Harper Dorn Creep

14
Flow of vacancies according to (a) Nabarro–Herring and (b) Coble mechanisms, resulting in an increase in the length of the specimen. Diffusion Creep

15
Dislocation climb (a) upwards, under compressive σ22 stresses, and (b) downwards, under tensile σ22 stresses. Dislocation Climb

16
Different regimes for diffusion creep in alumina; notice that cations (Al3+) and anions (O2−) have different diffusion coefficients, leading to different regimes of dominance. (From A. H. Chokshi and T. G. Langdon, Defect and Diffusion Forum, 66–69 (1989) 1205.) Diffusion Creep

17
Power relationship between ˙ε and σ for AISI 316 stainless steel. Adapted with permission from S. N. Monteiro and T. L. da Silveira, Metalurgia-ABM, 35 (1979) 327. Power Law Creep Dislocation (Power Law) Creep: 10^(-2) < σ/G < 10^(-4)

18
Dislocation overcoming obstacles by climb, according to Weertman theory. (a) Overcoming Cottrell–Lomer locks. (b) Overcoming an obstacle. Dislocations Overcoming Obstacles Weertman Mechanism

19
Shear stress vs. shear strain rate in an aluminum (6061) with 30 vol.% SiC particulate composite in creep. (From K.-T. Park, E. J. Lavernia, and F. A. Mohamed, Acta Met. Mater., 38 (1990) 2149.) Shear Stress and Shear Strain Rate

20
Effect of stress and temperature on deformation substructure developed in AISI 316 stainless steel in middle of stage II. Reprinted with permission from H.-J. Kestenbach, W. Krause, and T. L. da Silveira, Acta Met., 26 (1978) 661.) Dislocation Glide

21
(a) Steady-state grain-boundary sliding with diffusional accommodations. (b) Same process as in (a), in an idealized polycrystal; the dashed lines show the flow of vacancies. (Reprinted with permission from R. Raj and M. F. Ashby, Met. Trans., 2A (1971) 1113.) Grain Boundary Sliding

22
Grain-boundary sliding assisted by diffusion in Ashby–Verrall’s model. (Reprinted with permission from M. F. Ashby and R. A. Verrall, Acta Met., 21 (1973) 149.) Ashby-Verrall’s Model

23
Weertman–Ashby map for pure silver, established for a critical strain rate of 10−8 s−1; it can be seen how the deformation- mechanism fields are affected by the grain size. Adapted with permission from M. F. Ashby, Acta Met., 20 (1972) 887. Weertman-Ashby Map for Pure Silver

24
Weertman–Ashby map for tungsten, showing constant strain-rate contours. (Reprinted with permission from M. F. Ashby, Acta Met., 20 (1972) 887.) Weertman-Ashby Map for Tungsten

25
Weertman-Ashby Map for Al2O3

26
. (From W.D. Nix and J. C. Gibeling, in Flow and Fracture at ElevatedTemperatures, ed, R. Raj (Metals Park, Ohio: ASM, 1985).) Mechanisms of intergranular nucleation

27
Transmission electron micrograph of Mar M-200; notice the cuboidal γ precipitates. (Courtesy of L. E. Murr.) Heat-Resistance Materials

28
(Reprinted with from C. T. Sims and W. C. Hagel, eds., The Superalloys (New York: Wiley, 1972), p. 33.) Microstructural Strengthening Mechanism in nickel-based superalloys

29
Rafting in MAR M-200 monocrystalline superalloy; (a) original configuration of gamma prime precipitates aligned with three orthogonal cube axes; (b) creep deformed at 1253 K for 28 hours along the [010] direction, leading to coarsening of precipitates along loading direction. (From U. Glatzel, “Microstructure and Internal Strains of Undeformed and Creep Deformed Samples of a Nickel-Based Superalloy,” Habilitation Dissertation,Technische Universit¨at, Berlin, 1994.) Rafting

30
Stress versus temperatures curves for rupture in 1,000 hours for selected nickel-based superalloys. (Reprinted with permission from C. T. Sims and W. C. Hagel, eds., The Superalloys (New York: Wiley, 1972), p. vii.) Stress-Rupture (at 1000 hours) vs. Temperature for Heat Resistant Materials

31
Cross-section of a gas turbine showing different parts. The temperature of gases in combustion chamber reaches 1500 ◦C. Gas Turbine

32
(a) Single crystal turbine blade developed for stationary turbine. (Courtesy of U. Glatzel.) (b) Evolution of maximum temperature in gas turbines; notice the significant improvement made possible by the introduction of thermal barrier coatings (TBCs). (Courtesy of V. Thien, Siemens.) Turbine Blade

33
Spring–dashpot analogs (a) in series and (b) in parallel. Creep in Polymers

34
(a)Strain–time and (b) stress–time predictions for Maxwell and Voigt models. Maxwell and Voigt Models

35
Strain response as a function of time for a glassy, viscoelastic polymer subjected to a constant stress σ0. Increasing the molecular weight or degree of cross-linking tends to promote secondary bonding between chains and thus make the polymer more creep resistant. Viscoelastic Polymer

36
(a) A series of creep compliances vs. time, both on logarithmic scales, over a range of temperature. (b) The individual plots in (a) can be superposed by horizontal shifting (along the log-time axis) by an amount log aT, to obtain a master curve corresponding to a reference temperature Tg of the polymer. (c) Shift along the log- time scale to produce a master curve. (Courtesy of W. Knauss.) (d) “Experimentally” determined shift factor. Creep Compliances

37
A constant imposed strain ε0 results in a drop in stress σ(t) as a function of time. Stress Relaxation

38
A master curve obtained in the case of stress relaxation, showing the variation in the reduced modulus as a function of time. Also shown is the effect of cross-linking and molecular weight. Effect of Crosslinking on Stress Relaxation

39
Metal interconnect line covered by passivation layer subjected toelectromigration; (a) overall scheme; (b) voids and cracks produced by thermal mismatch and electromigration; (c) basic scheme used in Nix Arzt equation, which assumes grain-boundary diffusion of vacancies counterbalancing electron wind. (Adapted from W. D. Nix and E. Arzt. Met. Trans., 23A (1992) 2007.) Electromigration

40
Superplastic tensile deformation in Pb–62% Sn eutectic alloy tested at 415 K and a strain rate of 1.33 × 10−4 s−1; total strain of 48.5. (From M. M. I. Ahmed and T. G. Langdon, Met. Trans. A, 8 (1977) 1832.) Superplasticity

41
(a) Schematic representation of plastic deformation in tension with formation and inhibition of necking. (b) Engineering-stress– engineering-strain curves. Plastic Deformation

42
Strain-rate dependence of (a) stress and (b) strain-rate sensitivity for Mg–Al eutectic alloy tested at 350 ◦C (grain size 10 μm). (After D. Lee, Acta. Met., 17 (1969) 1057.) Strain Rate Dependence

43
Tensile fracture strain and stress as a function of strain rate for Zr–22% Al alloy with 2.5-μm grain size. (After F. A. Mohamed, M. M. I. Ahmed, and T. G. Langdon, Met. Trans. A, 8 (1977) 933.) Fracture

44
Effect of strain-rate sensitivity m on maximum tensile elongation for different alloys (Fe, Mg, Pu, Pb–Sr, Ti, Zn, Zr based). (From D. M. R. Taplin, G. L. Dunlop, and T. G. Langdon, Ann. Rev. Mater. Sci., 9 (1979) 151.) Effect of Strain Rate Sensitivity

45
Cavitation in superplasticity formed 7475-T6 aluminum alloy (ε = 3.5) at 475 ◦C and 5 × 10−4 s−1. (a) Atmospheric pressure. (b) Hydrostatic pressure P = 4 MPa. (Courtesy of A. K. Mukherjee.) Cavitation in Superplasticity

46
(a) Effect of grain size on elongation: (A) Initial configuration. (B) Large grains. (C) Fine grains (10 μm) (Reprinted with permission from N. E. Paton, C. H. Hamilton, J. Wert, and M. Mahoney, J. Metal, 34 (1981) No. 8, 21.) (b) Failure strains increase with superimposed hydrostatic pressure (from 0 to 5.6 MPa). (Courtesy of A. K. Mukherjee.) Effect of Grain Size on Elongation

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google